Oct 6, 2017 - This is an open access article published under an ACS AuthorChoice License, which permits copying and redistribution of the article or any ...
This is an open access article published under an ACS AuthorChoice License, which permits copying and redistribution of the article or any adaptations for non-commercial purposes.
Core−Shell Nanoparticles as an Eﬃcient, Sustained, and Triggered Drug-Delivery System Sonal Deshpande,† Sapna Sharma,† Veena Koul,†,‡ and Neetu Singh*,†,‡ †
Centre for Biomedical Engineering, Indian Institute of Technology-Delhi, Hauz Khas, New Delhi 110016, India Biomedical Engineering Unit, All India Institute of Medical Sciences, Ansari Nagar, New Delhi 110029, India
S Supporting Information *
ABSTRACT: One of the challenges in designing a successful drug-delivery vehicle is the control over drug release. Toward this, a number of multifunctional nanoparticles with multiple triggers and complex chemistries have been developed. To achieve an eﬃcient and maximum therapeutic eﬀect, a trigger dependent drug-delivery system with sustained release is desirable. In this paper, we report the use of a combination of thermoresponsive gold core and polymeric shell nanoparticles that can provide a sustained, triggered release of doxorubicin, making the system more eﬃcient compared to individual nanoparticles. The selection of the system was dependent on the best trigger applicable in biological systems and a component responsive to that trigger. Because of the best tissue penetration depth observed for radiofrequency (rf), we chose rf as a trigger. Whereas the gold nanoparticles (AuNPs) provided hyperthermia trigger on exposure to rf ﬁelds, the thermoresponsiveness was endowed by poly(N-isopropylacrylamide) (pNIPAm)-based polymer shells. AuNPs with three diﬀerent compositions of shells, only pNIPAm and p(NIPAm-co-NIPMAm) with the ratio of NIPAm/N-(isopropylmethacrylamide) (NIPMAm) 1:1 (pNIPMAm50) and 1:3 (pNIPMAm75), were synthesized. We observed that the polymer coating on the AuNPs did not aﬀect the heating eﬃciency of AuNPs by rf and exhibited a temperature-dependent release of the chemotherapeutic drug, doxorubicin. The nanoparticles were biocompatible, stable in biologically relevant media, and were able to show a burst as well as a sustained release, which was rf-dependent. Interestingly, we observed that when HeLa cells were treated with doxorubicin-loaded gold core−polymeric shell NPs and exposed to rf for varying times, the mixture of the two polymeric shell nanoparticles induced more cell death as compared to the cells treated with single nanoparticles, suggesting that such multi-nanoparticle systems can be more eﬃcacious delivery systems instead of a single multicomponent system.
INTRODUCTION Conventional drug therapy, though eﬀective, mostly requires periodic administration of drugs at concentrations higher than that required at the target site, which can result in systemic toxicity. Moreover, its eﬀectiveness is also highly dependent on patient compliance. To decrease the frequency of administration, dependence on patient compliance, and enhancing the eﬀective concentration of the drug at the target site, nanocarriers are being exploited for drug delivery.1,2 The basic properties considered while designing the nanocarriers are biocompatibility, drug-loading capacity, chemical handles for bioconjugation of targeting moieties, and control over the release kinetics of loaded drugs. Most of the nanocarriers developed for drug delivery show a sustained release, where the release is governed by Fickian diﬀusion,3 thereby providing least control over the release. Further eﬀorts have led to the next generation “smart” nanocarriers, in which the release can be triggered in response to an endogenous or exogenous stimulus. The endogenous stimuli, such as pH,4−6 redox,7−9 hypoxia,10 and enzymes,11,12 © 2017 American Chemical Society
are based on the microenvironment speciﬁc to the target sites. Because these triggers are continuously “ON”, once activated, the system shows a continuous release. Alternatively, the exogenous triggers, such as temperature,13 light,14,15 magnetic ﬁeld,16 and electric current,17 can provide advanced release proﬁles, also known as “on demand” release that follows “ON− OFF” signals. In fact, till date, a number of such nanocarriers, especially for delivery of nucleic acids, have been reported.18 These systems utilize the diﬀerence in melting temperatures of diﬀerent nucleic acid sequences for delivery, thereby making their application highly speciﬁc to nucleic acids.19 Similarly, other systems such as nanogels are also being developed as switchable drug-delivery systems.20,21 In the case of nanogels, where the release is dependent on deswelling and swelling properties, on exposure to the stimuli, most of the drug gets released from the system, thereby resulting in availability of a Received: July 18, 2017 Accepted: September 25, 2017 Published: October 6, 2017 6455
DOI: 10.1021/acsomega.7b01016 ACS Omega 2017, 2, 6455−6463
Figure 1. (a) Absorbance spectra of AuNPs and core−shells. (b) Transmission electron micrograph of AuNP−pNIPAm core−shell. Inset: Magniﬁed image of the core−shell (scale = 10 nm). (c) Hydrodynamic diameter of the nanoparticles as measured by dynamic light scattering (DLS). (d) Zeta potential of the nanoparticles. (e) Eﬀect of temperature on the hydrodynamic diameter of the core−shells analyzed by DLS. The error bars indicate the standard deviation between the triplicates. pNIPAm: Au core with the pNIPAm shell; pNIPMAm50 and pNIPMAm75: Au core with p(NIPAmco-NIPMAm) shells with NIPAm/NIPMAm in the ratio of 1:1 and 1:3, respectively.
(NIPMAm), and so forth in the polymer backbone.25 However, as the use of acids as a co-monomer also confers pH responsiveness to the nanogel, we selected NIPMAm for the shell synthesis. Though the biocompatibility of pNIPAm is one of the concerns limiting its clinical translation, it has been wellestablished that the toxicity observed in these systems is due to the monomer.26 In fact, the polymer has been shown to be biocompatible at concentrations relevant to many biomedical applications. On the other hand, AuNPs are widely accepted for biomedical applications because of their bioinertness and biocompatibility.2,27,28 They exhibit excellent optical resonance of their surface plasmons, resulting in strong absorbance at a characteristic wavelength and conversion of the resonance energy into heat. Although gold nanorods with surface plasmon resonance in the near-infrared (NIR) region have shown potential, their practical implementation is limited by the extent of tissue penetration (